Toughness is a mechanical term that is used in several contexts; loosely speaking,
it is a measure of the ability of a material to absorb energy up to fracture. Specimen geometry as well as the manner of load application are important in toughness determinations. For dynamic (high strain rate) loading conditions and when a notch (or point of stress concentration) is present, notch toughness is assessed by using an impact test, as discussed in Section 9.8. Furthermore, fracture toughness is a property indicative of a material’s resistance to fracture when a crack is present (Section 9.5).
For the static (low strain rate) situation, toughness may be ascertained from the results of a tensile stress–strain test. It is the area under the–⑀curve up to the point of fracture. The units for toughness are the same as for resilience (i.e., energy per unit volume of material). For a material to be tough, it must display both strength and ductility; and often, ductile materials are tougher than brittle ones. This is demonstrated in Figure 7.13, in which the stress–strain curves are plotted for both material types. Hence, even though the brittle material has higher yield and tensile strengths, it has a lower toughness than the ductile one, by virtue of lack of ductility; this is deduced by comparing the areas ABC and AB⬘C⬘ in Figure 7.13.
From Figure 7.11, the decline in the stress necessary to continue deformation past the maximum, point M, seems to indicate that the metal is becoming weaker. This is not at all the case; as a matter of fact, it is increasing in strength. However, the cross-sectional area is decreasing rapidly within the neck region, where deformation is occurring. This results in a reduction in the load-bearing capacity of the specimen. The stress, as computed from Equation 7.1, is on the basis of the original cross- sectional area before any deformation, and does not take into account this diminu- tion in area at the neck.
Sometimes it is more meaningful to use a true stress–true strain scheme. True
Aiover which deformation is occurring (i.e., the neck, past the tensile point), or
T⫽ F Ai
Furthermore, it is occasionally more convenient to represent strain as true
strain⑀T, defined by
⑀T⫽ln li l0
If no volume change occurs during deformation, that is, if
true and engineering stress and strain are related according to
T⫽ (1⫹ ⑀) (7.18a)
⑀T⫽ ln(1⫹ ⑀) (7.18b)
Equations 7.18a and 7.18b are valid only to the onset of necking; beyond this point true stress and strain should be computed from actual load, cross-sectional area, and gauge length measurements.
A schematic comparison of engineering and true stress–strain behavior is made in Figure 7.16. It is worth noting that the true stress necessary to sustain increasing strain continues to rise past the tensile point M⬘.
Coincident with the formation of a neck is the introduction of a complex stress state within the neck region (i.e., the existence of other stress components in addition to the axial stress). As a consequence, the correct stress (axial) within the neck is slightly lower than the stress computed from the applied load and neck cross- sectional area. This leads to the ‘‘corrected’’ curve in Figure 7.16.
For some metals and alloys the region of the true stress-strain curve from the onset of plastic deformation to the point at which necking begins may be approximated by
168 ● Chapter 7 / Mechanical Properties
Strain Engineering Corrected True M⬘ M Stress
FIGURE7.16 A comparison of typical tensile engineering stress–strain and true stress–strain behaviors. Necking begins at point M on the engineering curve, which corresponds to M⬘on the true curve. The ‘‘corrected’’ true stress–strain curve takes into account the complex stress state within the neck region.
7.7 True Stress and Strain ● 169
In this expression, K and n are constants, which values will vary from alloy to alloy, and will also depend on the condition of the material (i.e., whether it has been plastically deformed, heat treated, etc.). The parameter n is often termed the strain-
hardening exponent and has a value less than unity. Values of n and K for several
alloys are contained in Table 7.3.
A cylindrical specimen of steel having an original diameter of 12.8 mm (0.505 in.) is tensile tested to fracture and found to have an engineering fracture strengthfof 460 MPa (67,000 psi). If its cross-sectional diameter at fracture
is 10.7 mm (0.422 in.), determine:
(a) The ductility in terms of percent reduction in area. (b) The true stress at fracture.
SO L U T I O N
(a) Ductility is computed using Equation 7.12, as
冉12.8 mm 2
冉10.7 mm 2
冉12.8 mm 2
冊2 앟 ⫻100 ⫽128.7 mm2⫺89.9 mm2 128.7 mm2 ⫻100⫽30%
(b) True stress is defined by Equation 7.15, where in this case the area is taken
as the fracture area Af. However, the load at fracture must first be computed
Table 7.3 Tabulation of n and K Values (Equation 7.19) for
Material n MPa psi
Low-carbon steel 0.26 530 77,000 (annealed) Alloy steel 0.15 640 93,000 (Type 4340, annealed) Stainless steel 0.45 1275 185,000 (Type 304, annealed) Aluminum (annealed) 0.20 180 26,000 100,000 Aluminum alloy 0.16 690
(Type 2024, heat treated)
Copper (annealed) 0.54
Brass 0.49 895 130,000 (70Cu–30Zn, annealed)
Source: From Manufacturing Processes for Engineering Materials by
Seope Kalpakjian,1997. Reprinted by permission of Prentice-Hall, Inc., Upper Saddle River, NJ.
from the fracture strength as
Thus, the true stress is calculated as T⫽ F Af ⫽ 59,200 N (89.9 mm2)
冉1 m 2 106mm2
冊⫽6.6⫻108N/m2⫽660 MPa (95,700 psi)
Compute the strain-hardening exponent n in Equation 7.19 for an alloy in which a true stress of 415 MPa (60,000 psi) produces a true strain of 0.10; assume a value of 1035 MPa (150,000 psi) for K.
SO L U T I O N
This requires some algebraic manipulation of Equation 7.19 so that n becomes the dependent parameter. This is accomplished by taking logarithms and rear- ranging. Solving for n yields
⫽log(415 MPa)⫺log(1035 MPa)
Upon release of the load during the course of a stress–strain test, some fraction of the total deformation is recovered as elastic strain. This behavior is demonstrated in Figure 7.17, a schematic engineering stress–strain plot. During the unloading cycle, the curve traces a near straight-line path from the point of unloading (point
D), and its slope is virtually identical to the modulus of elasticity, or parallel to the
initial elastic portion of the curve. The magnitude of this elastic strain, which is regained during unloading, corresponds to the strain recovery, as shown in Figure 7.17. If the load is reapplied, the curve will traverse essentially the same linear portion in the direction opposite to unloading; yielding will again occur at the unloading stress level where the unloading began. There will also be an elastic strain recovery associated with fracture.
Of course, metals may experience plastic deformation under the influence of applied compressive, shear, and torsional loads. The resulting stress–strain behavior into
7.10 Flexural Strength ● 171
the plastic region will be similar to the tensile counterpart (Figure 7.10a: yielding and the associated curvature). However, for compression, there will be no maximum, since necking does not occur; furthermore, the mode of fracture will be different from that for tension.